Please copy and paste this embed script to where you want to embed

ARTICLE IN PRESS

Microelectronics Journal 37 (2006) 910–915 www.elsevier.com/locate/mejo

Hot-Probe method for evaluation of impurities concentration in semiconductors G. Golan, A. Axelevitch, B. Gorenstein, V. Manevych Holon Academic Institute of Technology, Israel Received 2 December 2005; accepted 29 January 2006 Available online 29 March 2006

Abstract Electrical, optical, and mechanical properties of thin ﬁlms signiﬁcantly differ from those of bulk materials. Therefore, characterization methods for evaluation of thin ﬁlm properties became highly important. A novel approach to the well known ‘‘Hot-Probe’’ method is proposed and applied in our work. The conventional Hot Probe characterization method enables only the deﬁnition of a semiconductor type, P or N, by identifying the majority charged carriers. According to the new Hot Probe technique, one can measure and calculate the majority charged carriers concentration and its dynamic parameters. Feasibility proof of the upgraded Hot Probe method was done in Si and Ge bulk, and in thin ﬁlm semiconductor samples. r 2006 Elsevier Ltd. All rights reserved. Keywords: Hot-Probe method; Charged carriers concentration; Type of charged carriers; Semiconductors ﬁlm properties

1. Introduction The conventional Hot-Probe experiment provides a simple yet efﬁcient way to distinguish between n-type and p-type semiconductors using a heated probe and a standard multimeter. The experiment is done by attaching a couple of cold probe and hot probe to a semiconductor surface. Both probes are wired to a sensitive electrometer [1]. The hot probe is connected to the positive terminal of the meter while the cold probe is connected to the negative terminal. While applying the cold and hot probes to an n-type semiconductor, positive voltage readout is obtained in the meter, whereas for a p-type semiconductor, negative voltage is obtained. A simple explanation for this experiment is that the thermally excited majority free charged carriers are translated within the semiconductor from the hot probe to the cold probe. The mechanism for this motion within the semiconductor is of a diffusion type since the material is uniformly doped due to the constant heating in the hot probe contact. These translated majority carriers deﬁne the electrical potential sign of the measured current in the Corresponding author.

E-mail address: [email protected] (A. Axelevitch). 0026-2692/$ - see front matter r 2006 Elsevier Ltd. All rights reserved. doi:10.1016/j.mejo.2006.01.014

multimeter. Thus, the hot probe surrounding zone becomes charged with minority carriers and the cold probe remains neutral [2]. Hot Probe experiment may be realized by three various methods: 1. To heat a probe and connect it to the sample under evaluation for a short period while keeping the second electrode (the cold one) constantly connected; variation of the multimeter to the positive or negative direction indicates type of the semiconductor (the old ‘‘HotProbe’’ method). 2. To connect two electrodes to the sample under evaluation and heat one of them; this way we obtain information on the type of semiconductor as in the ﬁrst one and the thermo-electrical voltage dependence on temperature (Seebeck coefﬁcient). This is no matter of the present article. 3. To heat a mediator probe for a pre-deﬁned temperature and attach it to one of the two probes for a certain time. Two electrodes are constantly held attached to the surface. Attachment is maintained until a steady state is obtained. Then the mediator probe heater is removed from the heated electrode. In this way one gets

ARTICLE IN PRESS G. Golan et al. / Microelectronics Journal 37 (2006) 910–915

additional information concerning the majority charged carriers concentration and the dynamic parameters of the semiconductor material. In our actual work we concentrate efforts on the majority charged carriers concentration only. Dynamic parameters will be discussed in future research. Generally, the Hot-Probe measurement may be related to as a three-step process. Firstly, the heated probe excites additional charged carriers which are the free charged carriers. This process is different for various materials and various temperatures. Secondly, the warmed majority carriers begin to run from the heated point by a diffusion mechanism. Simultaneously, a built-in electrical ﬁeld is created between the electrodes. At the same time, the second (cold) electrode also warms. This warming and the built-in electrical ﬁeld tend to prevent the diffusion process up to a halt at a steady state. This steady state condition carries on until the heat source is disconnected from the electrode. Thirdly, recombination processes of the charged carriers are performed after removal of the heat source. The above three-step process may be described, in general, by the continuity and Poisson’s equations [3]: 8 qQ > > < rJ þ qt ¼ 0; (1) Q > > : : rE ¼ e0 er Here Q is the uncompensated charge density excited by the heated electrode, J is the current density, e0 and er are the absolute and relative permittivity, and E is the built-in electrical ﬁeld. For a theoretical consideration we assume that the semiconductor bulk or thin ﬁlm samples are positioned on top of a dielectric substrate and they are randomly doped with isotropic properties. Such as a semiconductor includes two different types of charged carriers: negative and positive, the continuity equation and the Poisson’s equation may be divided on two different equations according to the relation: Q ¼ ðp nÞq,

(2)

where p and n are positive and negative charged carriers consequently, and q is an elementary charge. Before heating (the steady state), the semiconductor sample is in a compensated electro-neutral state, according to the electro-neutrality rule n þ N A ¼ p þ N D,

(3)

where NA is the concentration of acceptor ions and ND is the concentration of donor ions. In the case of extrinsic semiconductor, a p-type for example, the ND value may be neglected and using the charge conservation law ðpn ¼ n2i Þ, Eq. (3) transforms into the following form p ¼ n þ N A ¼ n2i =p þ N A ,

(4)

where ni ¼ pi is the intrinsic charged carriers concentration at normal temperature (300 K). The solution of this

equation will be sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2 NA NA þ n2i . p¼ 2 2

911

(5)

At higher temperatures, the majority carrier concentration will be differed from (5) on the value niT only, where niT ¼ piT is the intrinsic concentration at T temperature. Heating in one point situated in a distance x from the second (cool) point creates the novel majority carriers concentration pT. The difference ðpT pÞ ¼ ðnT 2nÞ ¼ Dp ¼ Dn appears to be the thermally excited charge density. These additional charged carriers together with heated majority carriers diffuse from heated electrode area to all directions result in creation of voltage difference. The value Dp ¼ Dn may be presented as follows: sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2 2 NA NA Dn ¼ (6) þ n2iT þ n2i . 2 2 Let us assume that the effective mass of the charged carriers and a semiconductor bandgap are stable at the temperature variation from room temperature of up to about 150 1C. So, the intrinsic charged carriers concentration at increased temperature will rise as follows [4]: Eg 3=2 niT ¼ AT exp (7) 2kT where A is the proportionality coefﬁcient, Eg is a bandgap of the semiconductor, and k is the Boltzmann’s constant. This value may be presented using a tabular or known intrinsic concentration at the normal temperature: 3=2 Eg T T0 niT ¼ ni exp 1 ¼ ni R and T0 2kT 0 T 3=2 Eg T T0 exp 1 R¼ , ð8Þ T0 2kT 0 T where R is a function of the heating temperature. Thus, Eq. (6) may be rewritten in the following way: sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2 2 NA NA (9) þ n2i R2 þ n2i . Dn ¼ Dp ¼ 2 2 This equation may be approximately solved for NA. Such as Dnoni oniR in our assumptions, one can neglect small values and the solution we obtain is in the following form: NA

n2i R2 . Dn

(10)

This equation enables an approximate estimation of the impurities concentration in the semiconductor or thin ﬁlm if measured the additional charge Q. Evidently, the same formula will be obtained for an n-type semiconductor material. This estimation may be veriﬁed by an independent measurement of the material resistivity. The main goal of the present work is to prove the proposed theory and apply it to practical measurements.

ARTICLE IN PRESS 912

G. Golan et al. / Microelectronics Journal 37 (2006) 910–915

2. Experimental details The experimental laboratory setup is shown in Fig. 1. Two spring-loaded Au-coated electrodes placed at a distance of L ¼ 10 mm from each other create the closed loop circuit with the digital multimeter. A thermo-couple equipped heater is attached to one of the electrodes to warm it up to 150 1C. A ‘‘WS 81’’ soldering iron of Weller was used also as heater and created a stable controllable temperature up to 450 1C. Voltage and current measurements were carried out using a Keithley automatic test station. The sheet resistance of all samples was measured using a conventional four-point probe station of Cascade Microtech. Silicon and germanium crystalline samples and germanium thin semiconductor ﬁlms doped with aluminum were studied in the experiment. Germanium thin ﬁlms were deposited by thermal evaporation. Aluminum powder was attached to the germanium to provide deposition of doped semiconductor coatings. In order to obtain a good Ohmic contact between the electrodes and the sample surface, we used an In–Ga eutectic grout. The measurement technique was as follows: A hot electrode was connected to the positive input of a digital voltmeter. Then, the hot electrode was heated up to the required temperature and attached to the sample surface. Measurement was done for 40–60 s approximately

and all readouts were stored and analyzed in the computerized Multi Log 710 multimeter of ‘‘ExTech’’. A current within the closed loop circuit of: multimeter, hot probe, semiconductor ﬁlm, cold probe and multimeter, is created due to a concentration drop of free charged carriers which generate diffusion within the sample due to the hot probe. There are two optional cases for such closed loops: (a) Ohmic contact between the probe electrodes and the sample surface, (b) blocking contact. In the ﬁrst case, current is measured and follows the polarities of the measured voltage. In the second case, closed circuit appears as a two back to back diodes pair. Thus, the current is deﬁned by backward saturation current only [5]. The value of this reversed current is very small and cannot be measured by conventional techniques. 3. Results As the distance of 10 mm between the hot and cold probes is not sufﬁciently high, the hot electrode conducts heat toward the cold probe on top of the surface plane. In order to check this temperature inﬂuence on the second electrode we measured simultaneously the temperatures in both positions of the hot electrode and cold electrode by independent thermo-couple temperature sensors. Fig. 2 presents the obtained temperature characteristics of the cold electrode in various processing times. It can be seen that maximum temperature at the second electrode (cold probe) after 40 s has not exceeded more than 30 1C, for the highest possible temperature of the hot electrode (450 1C). In lower temperatures, this difference was lower and for 150 1C on the hot electrode, the cold probe temperature was no more of 10 1C. Generally, the maximal variation of the cold point temperature was not more than 6.7% from other hot-probe temperature. Therefore, we may assume that the second electrode temperature deviation can be neglected in the initial stage of measurements and it must be considered farther. Fig. 3 presents a hot probe characteristics family of curves, measured in a germanium sample for various Measurement

Cold electrode temperature,°C

60

200°C

55

250°C

50

300°C 45

350°C

40

400°C

35

450°C

30 25 0

Fig. 1. Experimental laboratory setup for a hot-probe measurement.

150°C

20

40

60

80 100 Time, sec

120

140

160

Fig. 2. Cold electrode temperature while measurement.

ARTICLE IN PRESS 50 45 40 35 30 25 20 15 10 5 0

18

913

(6.8, 16.05) Steady state

16

150°C 200°C 250°C 300°C 400°C

0

Measured voltage, mV

Measured voltage, mV

G. Golan et al. / Microelectronics Journal 37 (2006) 910–915

14 Temperature 150° C

12 10 8 6

(1.2, 0.01) Initial state

4 2

10 20 30 40 50 60 70 80 90 100 110 120

0

Processing time, sec

2

0 Fig. 3. Hot-probe characteristics for n-type germanium in various temperatures.

6

4

8

10

Time,sec Fig. 4. Hot-probe characteristic of germanium, measured at 150 1C.

Si thickness is of 1 mm

Measured voltage, mV

-40 -35 -30 -25 -20

100° C

-15

120° C

-10 -5 0 0

10

20

30 40 50 60 70 Processing time, sec

80

90 100

Fig. 5. Averaged hot-probe characteristics for p-type silicon sample.

poly-Si thickness is of 0.7 mm

0

-5 -10 -10 -15

-20

voltage current

-20

-30

Measured current, µA

0 Measured viltage, mV

temperatures of the hot electrode. These curves show a positive voltage measured between the two electrodes. Therefore, we conclude that the majority carriers in the Ge sample under evaluation are electrons. In other words, this is an n-type semiconductor. The characteristic measurements were repeated for various temperatures. The temperature inﬂuence on the obtained curves are found as follows: by increasing the hot-probe temperature, the measured voltage between electrodes was also increased. All curves are similar to each other. Three different regions may be distinguished in the obtained characteristics: (a) a steep rise at the ﬁrst part, (b) fast decrease to an almost steady state which continues decreasing slowly, and (c) a sharp decrease after removing the heater from the electrode. The slope of voltage decrease in the middle part of the curves is inﬂuenced by the cold electrode temperature increase, in our opinion. It is interesting to note that the initial growth and the ﬁnal decay have the same slopes. This indicates an identity of both physical processes of generation and recombination. Fig. 4 presents an initial part of the hot-probe characteristic for a germanium chip measured at 150 1C. This ﬁgure demonstrates the relationship between the initial state and the steady state. Averaged hot-probe characteristics for a p-type mono-crystal silicon sample and for a p-type polycrystalline silicon sample are presented in Figs. 5 and 6. These characteristics are very similar for various crystal forms of silicon. Fig. 6 shows the voltage and current characteristics measured in the same sample. As shown, the voltage and current curves are almost of the same nature and the conductance of these samples is deﬁned by the conventional Ohm’s law. Hot-probe characteristics for germanium thin ﬁlms on glass substrates are presented in Fig. 7. These characteristics show measured voltages as a function of heating time for two different temperatures, and shows the same behavior of a semiconductor regardless its type. Obtained ﬁlms are of p-type and n-type as shown from the negative (a) and positive (b) values of the measured voltages. Increasing of aluminum in the precursor evaporating

Temperature 100 °C

-25 0

10

20 30 40 50 60 Processing time, sec

70

-40 80

Fig. 6. Averaged hot-probe characteristics for p-type polycrystalline silicon sample.

material changes the sign of the majority charge carriers in the grown germanium ﬁlm. Comparing hot-probe characteristics measured for bulk, and thin ﬁlm semiconductor materials (see Figs. 3, 5–7) demonstrates that these materials behave the same way irrespective of their crystal structure and/or thickness. Thus, the same measurement

ARTICLE IN PRESS G. Golan et al. / Microelectronics Journal 37 (2006) 910–915

914

Measured voltage, mV

0.0

Here D is the diffusion coefﬁcient of the charged carriers. Now, using the relation Q ¼ qNðx; tÞ the Poisson’s equation (1) takes the following form:

P-type germanium film.

-0.1

100° C

-0.2

qE q Q x2 pﬃﬃﬃﬃﬃﬃﬃﬃ exp ¼ . qx 2pe0 er pDt 4Dt

-0.3

If we designate

140° C

-0.4

B¼

-0.5 0

10

(a)

20 30 Processing time, sec

40

50

x2 4Dt

and

pﬃﬃﬃﬃﬃﬃ dx ¼ 2 Dt dy,

Eq. (13) becomes: (14)

which is a classic equation that cannot be solved using elementary functions [6]. However, the right part of Eq. (14) may be represented in a series form for yo1:

0.7 Measured voltage, mV

y2 ¼

qE 2 ¼ B ey qx

N-type germanium film.

0.8

q Q pﬃﬃﬃﬃﬃﬃﬃﬃ ; 2pe0 er pDt

(13)

0.6 0.5 0.4

2

ey ¼ 1

0.3 60° C 0.2 0.1 0.0

(b)

10

20 30 40 Processing time, sec

(15)

In our case, for x ¼ L ¼ 1 cm and a time of 5–10 s at temperatures of 300–423 K, yo1. Therefore, Eq. (14) may be integrated partially

100° C

0

y2 y4 y2n þ þ ð1Þ2 . 1! 2! n!

50

60

Fig. 7. Hot-probe characteristics for germanium thin ﬁlms doped with aluminum during deposition in glass substrates: (a) p-type ﬁlm, (b) n-type ﬁlm.

and calculation methods may be applied to characterize thin semiconductor ﬁlms regardless of the growth method.

E pﬃﬃﬃﬃﬃﬃ ¼ B 2 Dt

Z

y

2

ey dy ¼ By B 0

y3 1 y5 þB . 25 3

(16)

The voltage V measured between the hot probe and the cold probe may express from E by integration of the equation qV ¼ E. qx

(17)

Thus, (17) may be integrated using (16) as 4. Discussion The hot excited charged carriers begin diffusing from the hot probe at all directions meaning half sphere or 2p steradians. This diffusion process obeys the Fick law. In a constant heating temperature, the diffusion process resembles the diffusion from a deﬁned source. The hot charged carriers leave the heated zone and create a depletion region around the hot probe. Thus, the diffusion equation may be written in one-dimension as follows: Z 1 Nðx; tÞ dx ¼ Q, (11)

V y2 y4 pﬃﬃﬃﬃﬃﬃ ¼ B þ B . 2 12 2 Dt

(18)

After neglecting all small components and re-substitution, we obtain the following expression: V ¼

q Q x2 pﬃﬃﬃ . 2pe0 er p 4Dt

(19)

The additional charged carriers quantity may be obtained from this equation for x ¼ L:

0

where N(x,t) is a concentration of the free charged carriers in distance x and time t. The solution of Eq. (11) is in the well known Gaussian form: Q x2 Nðx; tÞ ¼ pﬃﬃﬃﬃﬃﬃﬃﬃ exp . 4Dt pDt

(12)

Q¼

V 2p3=2 e0 er 4Dt . qL2

(20)

In ﬁrst approximation, the diffusion coefﬁcient value may be calculated using the well known Einstein equation and tabular value of the charged carriers mobility for a given temperature. The sign of Dn is deﬁned by the type of

ARTICLE IN PRESS G. Golan et al. / Microelectronics Journal 37 (2006) 910–915

material. Calculations according to formulae (20) and (10) will obtain the majority charged carriers concentration. 5. Application of the hot probe method The type of the semiconductor material is deﬁned in the old ‘‘Hot-Probe’’ method by the sign of the measured voltage. A thermo-electric power (Seebeck’s coefﬁcient) may be calculated from measurements of the voltage at various temperatures. For example, in order to build the relationship of thermoelectric power and temperature, we use Fig. 3. Maximum value of the voltage should be related to the temperature. The angle of slope of the graphical characteristics is equal to the thermoelectric power. To estimate the majority charged carriers concentration, (8), (10) and (20) should be applied. Estimation of the majority charged carriers was done for Ge sample, n-type. Its hot-probe characteristic is presented in Fig. 4. As shown, the sample was measured by hot-probe at 150 1C. A time interval between the initial state and steady state was of 5.6 s, and the maximal measured voltage was 16.04 mV. Additional data for the Ge sample were taken from Ref. [7]: E g ¼ 0:66 eV, mn ¼ 3900 cm2 =V s, ni ¼ 2:4 1013 cm3 , er ¼ 16. Calculation accordingly presented theory results as the following values R ¼ 66:3, Dp 5 109 cm3 , and N D 2:5 1021 cm3 which agreed with a direct resistivity measurement.

915

6. Conclusion A novel approach to the well known hot-probe method was proposed. The novel approach consists of measurement of the thermo-generated voltage between heated and cold electrodes along a heating and relaxation periodic cycle. Obtained experimental curves are analyzed. Using mathematical results we are able to calculate the majority charged carries concentration in bulk semiconductors or thin ﬁlm semiconductors. It means that this renovated HotProbe method should become a prevalent method for operative evaluation of semi-conducting samples and semiconductor thin ﬁlms. References [1] B. Van Zeghbroeck, Principle of Semiconductor Devices, 1997, /http://ece-www.colorado.edu/bart/book/S. [2] A. Bar-Lev, G. Golan, Semiconductors, The Open University of Israel, Tel-Aviv, Israel, 1996 (Hebrew). [3] I.N. Volovichev, Yu.G. Gurevich, Generation and recombination in semiconductors, Semiconductors 35 (3) (2001) 306–315. [4] S.O. Kasap, Principle of Electrical Engineering Materials and Devices, McGraw Hill, Boston, 1997. [5] G. Golan, A. Axelevitch, B. Sigalov, B. Gorenstein, Investigation of phase transition mechanism in vanadium oxide thin ﬁlms, J. Optoelectronics Adv. Mat. 6 (1) (2004) 189–195. [6] G.M. Fihtengolz, Mathematical Analysis Fundamentals, GITTL, Moscow, 1957 (in Russian). [7] S.M. Sze, Physics of Semiconductor Devices, Wiley, New York, 1981.

View more...
Microelectronics Journal 37 (2006) 910–915 www.elsevier.com/locate/mejo

Hot-Probe method for evaluation of impurities concentration in semiconductors G. Golan, A. Axelevitch, B. Gorenstein, V. Manevych Holon Academic Institute of Technology, Israel Received 2 December 2005; accepted 29 January 2006 Available online 29 March 2006

Abstract Electrical, optical, and mechanical properties of thin ﬁlms signiﬁcantly differ from those of bulk materials. Therefore, characterization methods for evaluation of thin ﬁlm properties became highly important. A novel approach to the well known ‘‘Hot-Probe’’ method is proposed and applied in our work. The conventional Hot Probe characterization method enables only the deﬁnition of a semiconductor type, P or N, by identifying the majority charged carriers. According to the new Hot Probe technique, one can measure and calculate the majority charged carriers concentration and its dynamic parameters. Feasibility proof of the upgraded Hot Probe method was done in Si and Ge bulk, and in thin ﬁlm semiconductor samples. r 2006 Elsevier Ltd. All rights reserved. Keywords: Hot-Probe method; Charged carriers concentration; Type of charged carriers; Semiconductors ﬁlm properties

1. Introduction The conventional Hot-Probe experiment provides a simple yet efﬁcient way to distinguish between n-type and p-type semiconductors using a heated probe and a standard multimeter. The experiment is done by attaching a couple of cold probe and hot probe to a semiconductor surface. Both probes are wired to a sensitive electrometer [1]. The hot probe is connected to the positive terminal of the meter while the cold probe is connected to the negative terminal. While applying the cold and hot probes to an n-type semiconductor, positive voltage readout is obtained in the meter, whereas for a p-type semiconductor, negative voltage is obtained. A simple explanation for this experiment is that the thermally excited majority free charged carriers are translated within the semiconductor from the hot probe to the cold probe. The mechanism for this motion within the semiconductor is of a diffusion type since the material is uniformly doped due to the constant heating in the hot probe contact. These translated majority carriers deﬁne the electrical potential sign of the measured current in the Corresponding author.

E-mail address: [email protected] (A. Axelevitch). 0026-2692/$ - see front matter r 2006 Elsevier Ltd. All rights reserved. doi:10.1016/j.mejo.2006.01.014

multimeter. Thus, the hot probe surrounding zone becomes charged with minority carriers and the cold probe remains neutral [2]. Hot Probe experiment may be realized by three various methods: 1. To heat a probe and connect it to the sample under evaluation for a short period while keeping the second electrode (the cold one) constantly connected; variation of the multimeter to the positive or negative direction indicates type of the semiconductor (the old ‘‘HotProbe’’ method). 2. To connect two electrodes to the sample under evaluation and heat one of them; this way we obtain information on the type of semiconductor as in the ﬁrst one and the thermo-electrical voltage dependence on temperature (Seebeck coefﬁcient). This is no matter of the present article. 3. To heat a mediator probe for a pre-deﬁned temperature and attach it to one of the two probes for a certain time. Two electrodes are constantly held attached to the surface. Attachment is maintained until a steady state is obtained. Then the mediator probe heater is removed from the heated electrode. In this way one gets

ARTICLE IN PRESS G. Golan et al. / Microelectronics Journal 37 (2006) 910–915

additional information concerning the majority charged carriers concentration and the dynamic parameters of the semiconductor material. In our actual work we concentrate efforts on the majority charged carriers concentration only. Dynamic parameters will be discussed in future research. Generally, the Hot-Probe measurement may be related to as a three-step process. Firstly, the heated probe excites additional charged carriers which are the free charged carriers. This process is different for various materials and various temperatures. Secondly, the warmed majority carriers begin to run from the heated point by a diffusion mechanism. Simultaneously, a built-in electrical ﬁeld is created between the electrodes. At the same time, the second (cold) electrode also warms. This warming and the built-in electrical ﬁeld tend to prevent the diffusion process up to a halt at a steady state. This steady state condition carries on until the heat source is disconnected from the electrode. Thirdly, recombination processes of the charged carriers are performed after removal of the heat source. The above three-step process may be described, in general, by the continuity and Poisson’s equations [3]: 8 qQ > > < rJ þ qt ¼ 0; (1) Q > > : : rE ¼ e0 er Here Q is the uncompensated charge density excited by the heated electrode, J is the current density, e0 and er are the absolute and relative permittivity, and E is the built-in electrical ﬁeld. For a theoretical consideration we assume that the semiconductor bulk or thin ﬁlm samples are positioned on top of a dielectric substrate and they are randomly doped with isotropic properties. Such as a semiconductor includes two different types of charged carriers: negative and positive, the continuity equation and the Poisson’s equation may be divided on two different equations according to the relation: Q ¼ ðp nÞq,

(2)

where p and n are positive and negative charged carriers consequently, and q is an elementary charge. Before heating (the steady state), the semiconductor sample is in a compensated electro-neutral state, according to the electro-neutrality rule n þ N A ¼ p þ N D,

(3)

where NA is the concentration of acceptor ions and ND is the concentration of donor ions. In the case of extrinsic semiconductor, a p-type for example, the ND value may be neglected and using the charge conservation law ðpn ¼ n2i Þ, Eq. (3) transforms into the following form p ¼ n þ N A ¼ n2i =p þ N A ,

(4)

where ni ¼ pi is the intrinsic charged carriers concentration at normal temperature (300 K). The solution of this

equation will be sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2 NA NA þ n2i . p¼ 2 2

911

(5)

At higher temperatures, the majority carrier concentration will be differed from (5) on the value niT only, where niT ¼ piT is the intrinsic concentration at T temperature. Heating in one point situated in a distance x from the second (cool) point creates the novel majority carriers concentration pT. The difference ðpT pÞ ¼ ðnT 2nÞ ¼ Dp ¼ Dn appears to be the thermally excited charge density. These additional charged carriers together with heated majority carriers diffuse from heated electrode area to all directions result in creation of voltage difference. The value Dp ¼ Dn may be presented as follows: sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2 2 NA NA Dn ¼ (6) þ n2iT þ n2i . 2 2 Let us assume that the effective mass of the charged carriers and a semiconductor bandgap are stable at the temperature variation from room temperature of up to about 150 1C. So, the intrinsic charged carriers concentration at increased temperature will rise as follows [4]: Eg 3=2 niT ¼ AT exp (7) 2kT where A is the proportionality coefﬁcient, Eg is a bandgap of the semiconductor, and k is the Boltzmann’s constant. This value may be presented using a tabular or known intrinsic concentration at the normal temperature: 3=2 Eg T T0 niT ¼ ni exp 1 ¼ ni R and T0 2kT 0 T 3=2 Eg T T0 exp 1 R¼ , ð8Þ T0 2kT 0 T where R is a function of the heating temperature. Thus, Eq. (6) may be rewritten in the following way: sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 2 2 NA NA (9) þ n2i R2 þ n2i . Dn ¼ Dp ¼ 2 2 This equation may be approximately solved for NA. Such as Dnoni oniR in our assumptions, one can neglect small values and the solution we obtain is in the following form: NA

n2i R2 . Dn

(10)

This equation enables an approximate estimation of the impurities concentration in the semiconductor or thin ﬁlm if measured the additional charge Q. Evidently, the same formula will be obtained for an n-type semiconductor material. This estimation may be veriﬁed by an independent measurement of the material resistivity. The main goal of the present work is to prove the proposed theory and apply it to practical measurements.

ARTICLE IN PRESS 912

G. Golan et al. / Microelectronics Journal 37 (2006) 910–915

2. Experimental details The experimental laboratory setup is shown in Fig. 1. Two spring-loaded Au-coated electrodes placed at a distance of L ¼ 10 mm from each other create the closed loop circuit with the digital multimeter. A thermo-couple equipped heater is attached to one of the electrodes to warm it up to 150 1C. A ‘‘WS 81’’ soldering iron of Weller was used also as heater and created a stable controllable temperature up to 450 1C. Voltage and current measurements were carried out using a Keithley automatic test station. The sheet resistance of all samples was measured using a conventional four-point probe station of Cascade Microtech. Silicon and germanium crystalline samples and germanium thin semiconductor ﬁlms doped with aluminum were studied in the experiment. Germanium thin ﬁlms were deposited by thermal evaporation. Aluminum powder was attached to the germanium to provide deposition of doped semiconductor coatings. In order to obtain a good Ohmic contact between the electrodes and the sample surface, we used an In–Ga eutectic grout. The measurement technique was as follows: A hot electrode was connected to the positive input of a digital voltmeter. Then, the hot electrode was heated up to the required temperature and attached to the sample surface. Measurement was done for 40–60 s approximately

and all readouts were stored and analyzed in the computerized Multi Log 710 multimeter of ‘‘ExTech’’. A current within the closed loop circuit of: multimeter, hot probe, semiconductor ﬁlm, cold probe and multimeter, is created due to a concentration drop of free charged carriers which generate diffusion within the sample due to the hot probe. There are two optional cases for such closed loops: (a) Ohmic contact between the probe electrodes and the sample surface, (b) blocking contact. In the ﬁrst case, current is measured and follows the polarities of the measured voltage. In the second case, closed circuit appears as a two back to back diodes pair. Thus, the current is deﬁned by backward saturation current only [5]. The value of this reversed current is very small and cannot be measured by conventional techniques. 3. Results As the distance of 10 mm between the hot and cold probes is not sufﬁciently high, the hot electrode conducts heat toward the cold probe on top of the surface plane. In order to check this temperature inﬂuence on the second electrode we measured simultaneously the temperatures in both positions of the hot electrode and cold electrode by independent thermo-couple temperature sensors. Fig. 2 presents the obtained temperature characteristics of the cold electrode in various processing times. It can be seen that maximum temperature at the second electrode (cold probe) after 40 s has not exceeded more than 30 1C, for the highest possible temperature of the hot electrode (450 1C). In lower temperatures, this difference was lower and for 150 1C on the hot electrode, the cold probe temperature was no more of 10 1C. Generally, the maximal variation of the cold point temperature was not more than 6.7% from other hot-probe temperature. Therefore, we may assume that the second electrode temperature deviation can be neglected in the initial stage of measurements and it must be considered farther. Fig. 3 presents a hot probe characteristics family of curves, measured in a germanium sample for various Measurement

Cold electrode temperature,°C

60

200°C

55

250°C

50

300°C 45

350°C

40

400°C

35

450°C

30 25 0

Fig. 1. Experimental laboratory setup for a hot-probe measurement.

150°C

20

40

60

80 100 Time, sec

120

140

160

Fig. 2. Cold electrode temperature while measurement.

ARTICLE IN PRESS 50 45 40 35 30 25 20 15 10 5 0

18

913

(6.8, 16.05) Steady state

16

150°C 200°C 250°C 300°C 400°C

0

Measured voltage, mV

Measured voltage, mV

G. Golan et al. / Microelectronics Journal 37 (2006) 910–915

14 Temperature 150° C

12 10 8 6

(1.2, 0.01) Initial state

4 2

10 20 30 40 50 60 70 80 90 100 110 120

0

Processing time, sec

2

0 Fig. 3. Hot-probe characteristics for n-type germanium in various temperatures.

6

4

8

10

Time,sec Fig. 4. Hot-probe characteristic of germanium, measured at 150 1C.

Si thickness is of 1 mm

Measured voltage, mV

-40 -35 -30 -25 -20

100° C

-15

120° C

-10 -5 0 0

10

20

30 40 50 60 70 Processing time, sec

80

90 100

Fig. 5. Averaged hot-probe characteristics for p-type silicon sample.

poly-Si thickness is of 0.7 mm

0

-5 -10 -10 -15

-20

voltage current

-20

-30

Measured current, µA

0 Measured viltage, mV

temperatures of the hot electrode. These curves show a positive voltage measured between the two electrodes. Therefore, we conclude that the majority carriers in the Ge sample under evaluation are electrons. In other words, this is an n-type semiconductor. The characteristic measurements were repeated for various temperatures. The temperature inﬂuence on the obtained curves are found as follows: by increasing the hot-probe temperature, the measured voltage between electrodes was also increased. All curves are similar to each other. Three different regions may be distinguished in the obtained characteristics: (a) a steep rise at the ﬁrst part, (b) fast decrease to an almost steady state which continues decreasing slowly, and (c) a sharp decrease after removing the heater from the electrode. The slope of voltage decrease in the middle part of the curves is inﬂuenced by the cold electrode temperature increase, in our opinion. It is interesting to note that the initial growth and the ﬁnal decay have the same slopes. This indicates an identity of both physical processes of generation and recombination. Fig. 4 presents an initial part of the hot-probe characteristic for a germanium chip measured at 150 1C. This ﬁgure demonstrates the relationship between the initial state and the steady state. Averaged hot-probe characteristics for a p-type mono-crystal silicon sample and for a p-type polycrystalline silicon sample are presented in Figs. 5 and 6. These characteristics are very similar for various crystal forms of silicon. Fig. 6 shows the voltage and current characteristics measured in the same sample. As shown, the voltage and current curves are almost of the same nature and the conductance of these samples is deﬁned by the conventional Ohm’s law. Hot-probe characteristics for germanium thin ﬁlms on glass substrates are presented in Fig. 7. These characteristics show measured voltages as a function of heating time for two different temperatures, and shows the same behavior of a semiconductor regardless its type. Obtained ﬁlms are of p-type and n-type as shown from the negative (a) and positive (b) values of the measured voltages. Increasing of aluminum in the precursor evaporating

Temperature 100 °C

-25 0

10

20 30 40 50 60 Processing time, sec

70

-40 80

Fig. 6. Averaged hot-probe characteristics for p-type polycrystalline silicon sample.

material changes the sign of the majority charge carriers in the grown germanium ﬁlm. Comparing hot-probe characteristics measured for bulk, and thin ﬁlm semiconductor materials (see Figs. 3, 5–7) demonstrates that these materials behave the same way irrespective of their crystal structure and/or thickness. Thus, the same measurement

ARTICLE IN PRESS G. Golan et al. / Microelectronics Journal 37 (2006) 910–915

914

Measured voltage, mV

0.0

Here D is the diffusion coefﬁcient of the charged carriers. Now, using the relation Q ¼ qNðx; tÞ the Poisson’s equation (1) takes the following form:

P-type germanium film.

-0.1

100° C

-0.2

qE q Q x2 pﬃﬃﬃﬃﬃﬃﬃﬃ exp ¼ . qx 2pe0 er pDt 4Dt

-0.3

If we designate

140° C

-0.4

B¼

-0.5 0

10

(a)

20 30 Processing time, sec

40

50

x2 4Dt

and

pﬃﬃﬃﬃﬃﬃ dx ¼ 2 Dt dy,

Eq. (13) becomes: (14)

which is a classic equation that cannot be solved using elementary functions [6]. However, the right part of Eq. (14) may be represented in a series form for yo1:

0.7 Measured voltage, mV

y2 ¼

qE 2 ¼ B ey qx

N-type germanium film.

0.8

q Q pﬃﬃﬃﬃﬃﬃﬃﬃ ; 2pe0 er pDt

(13)

0.6 0.5 0.4

2

ey ¼ 1

0.3 60° C 0.2 0.1 0.0

(b)

10

20 30 40 Processing time, sec

(15)

In our case, for x ¼ L ¼ 1 cm and a time of 5–10 s at temperatures of 300–423 K, yo1. Therefore, Eq. (14) may be integrated partially

100° C

0

y2 y4 y2n þ þ ð1Þ2 . 1! 2! n!

50

60

Fig. 7. Hot-probe characteristics for germanium thin ﬁlms doped with aluminum during deposition in glass substrates: (a) p-type ﬁlm, (b) n-type ﬁlm.

and calculation methods may be applied to characterize thin semiconductor ﬁlms regardless of the growth method.

E pﬃﬃﬃﬃﬃﬃ ¼ B 2 Dt

Z

y

2

ey dy ¼ By B 0

y3 1 y5 þB . 25 3

(16)

The voltage V measured between the hot probe and the cold probe may express from E by integration of the equation qV ¼ E. qx

(17)

Thus, (17) may be integrated using (16) as 4. Discussion The hot excited charged carriers begin diffusing from the hot probe at all directions meaning half sphere or 2p steradians. This diffusion process obeys the Fick law. In a constant heating temperature, the diffusion process resembles the diffusion from a deﬁned source. The hot charged carriers leave the heated zone and create a depletion region around the hot probe. Thus, the diffusion equation may be written in one-dimension as follows: Z 1 Nðx; tÞ dx ¼ Q, (11)

V y2 y4 pﬃﬃﬃﬃﬃﬃ ¼ B þ B . 2 12 2 Dt

(18)

After neglecting all small components and re-substitution, we obtain the following expression: V ¼

q Q x2 pﬃﬃﬃ . 2pe0 er p 4Dt

(19)

The additional charged carriers quantity may be obtained from this equation for x ¼ L:

0

where N(x,t) is a concentration of the free charged carriers in distance x and time t. The solution of Eq. (11) is in the well known Gaussian form: Q x2 Nðx; tÞ ¼ pﬃﬃﬃﬃﬃﬃﬃﬃ exp . 4Dt pDt

(12)

Q¼

V 2p3=2 e0 er 4Dt . qL2

(20)

In ﬁrst approximation, the diffusion coefﬁcient value may be calculated using the well known Einstein equation and tabular value of the charged carriers mobility for a given temperature. The sign of Dn is deﬁned by the type of

ARTICLE IN PRESS G. Golan et al. / Microelectronics Journal 37 (2006) 910–915

material. Calculations according to formulae (20) and (10) will obtain the majority charged carriers concentration. 5. Application of the hot probe method The type of the semiconductor material is deﬁned in the old ‘‘Hot-Probe’’ method by the sign of the measured voltage. A thermo-electric power (Seebeck’s coefﬁcient) may be calculated from measurements of the voltage at various temperatures. For example, in order to build the relationship of thermoelectric power and temperature, we use Fig. 3. Maximum value of the voltage should be related to the temperature. The angle of slope of the graphical characteristics is equal to the thermoelectric power. To estimate the majority charged carriers concentration, (8), (10) and (20) should be applied. Estimation of the majority charged carriers was done for Ge sample, n-type. Its hot-probe characteristic is presented in Fig. 4. As shown, the sample was measured by hot-probe at 150 1C. A time interval between the initial state and steady state was of 5.6 s, and the maximal measured voltage was 16.04 mV. Additional data for the Ge sample were taken from Ref. [7]: E g ¼ 0:66 eV, mn ¼ 3900 cm2 =V s, ni ¼ 2:4 1013 cm3 , er ¼ 16. Calculation accordingly presented theory results as the following values R ¼ 66:3, Dp 5 109 cm3 , and N D 2:5 1021 cm3 which agreed with a direct resistivity measurement.

915

6. Conclusion A novel approach to the well known hot-probe method was proposed. The novel approach consists of measurement of the thermo-generated voltage between heated and cold electrodes along a heating and relaxation periodic cycle. Obtained experimental curves are analyzed. Using mathematical results we are able to calculate the majority charged carries concentration in bulk semiconductors or thin ﬁlm semiconductors. It means that this renovated HotProbe method should become a prevalent method for operative evaluation of semi-conducting samples and semiconductor thin ﬁlms. References [1] B. Van Zeghbroeck, Principle of Semiconductor Devices, 1997, /http://ece-www.colorado.edu/bart/book/S. [2] A. Bar-Lev, G. Golan, Semiconductors, The Open University of Israel, Tel-Aviv, Israel, 1996 (Hebrew). [3] I.N. Volovichev, Yu.G. Gurevich, Generation and recombination in semiconductors, Semiconductors 35 (3) (2001) 306–315. [4] S.O. Kasap, Principle of Electrical Engineering Materials and Devices, McGraw Hill, Boston, 1997. [5] G. Golan, A. Axelevitch, B. Sigalov, B. Gorenstein, Investigation of phase transition mechanism in vanadium oxide thin ﬁlms, J. Optoelectronics Adv. Mat. 6 (1) (2004) 189–195. [6] G.M. Fihtengolz, Mathematical Analysis Fundamentals, GITTL, Moscow, 1957 (in Russian). [7] S.M. Sze, Physics of Semiconductor Devices, Wiley, New York, 1981.

Thank you for interesting in our services. We are a non-profit group that run this website to share documents. We need your help to maintenance this website.

To keep our site running, we need your help to cover our server cost (about $400/m), a small donation will help us a lot.